28 February 2023

AperTO - Archivio Istituzionale Open Access dell'Università di Torino

*Original Citation:*

**Modeling and simulation in tribology across scales: An overview**

*Published version:*

DOI:10.1016/j.triboint.2018.02.005
*Terms of use:*

Open Access

(Article begins on next page)

Anyone can freely access the full text of works made available as "Open Access". Works made available under a Creative Commons license can be used according to the terms and conditions of said license. Use of all other works requires consent of the right holder (author or publisher) if not exempted from copyright protection by the applicable law.

*Availability:*

**This is the author's manuscript**

This version is available http://hdl.handle.net/2318/1673214 since 2018-08-12T22:25:55Z

1

**Modeling and Simulation in Tribology Across Scales: an ** **Overview **

A.I. Vakis, V.A. Yastrebov, J. Scheibert, L. Nicola, D. Dini, C. Minfray, A. Almqvist, M. Paggi, S.

Lee, G. Limbert, J.F. Molinari, G. Anciaux, S. Echeverri Restrepo, A. Papangelo, A. Cammarata, P.

Nicolini, R. Aghababaei, C. Putignano, S. Stupkiewicz, J. Lengiewicz, G. Costagliola, F. Bosia, R.

Guarino, N.M. Pugno, G. Carbone, M.H. Müser and M. Ciavarella*

**A.I. Vakis **

Advanced Production Engineering, Engineering and Technology Institute Groningen, Faculty of Science and Engineering, University of Groningen, Nijenborg 4, 9747 AG Groningen, the Netherlands

**V.A. Yastrebov **

MINES ParisTech, PSL Research University, Centre des Matériaux, CNRS UMR 7633, BP 87, F 91003 Evry, France

**J. Scheibert and C. Minfray **

Laboratoire de Tribologie et Dynamique des Systèmes, UMR5513, CNRS/Ecole Centrale de Lyon/Univ

Lyon/ENISE/ENTPE, 36 Avenue Guy de Collongue, F-69134 Ecully, France

**L. Nicola **

Department of Materials Science and Engineering, Delft University of Technology, Mekelweg 2, 2628 CD Delft, The Netherlands; Department of Industrial Engineering, University of Padova, via Venezia 1, 35015 Padua, Italy

**D. Dini **

Tribology Group, Department of Mechanical Engineering, Imperial College London, South Kensington Campus, Exhibition Road, London SW7 2AZ, UK

**A. Almqvist **

Division of Machine Elements, Luleå University of Technology, Luleå, Sweden

**M. Paggi **

IMT School for Advanced Studies Lucca, Multi-scale Analysis of Materials Research Unit, Piazza San Francesco 19, 55100 Lucca, Italy

**S. Lee **

Department of Mechanical Engineering, Technical University of Denmark, DK-2800, Kgs. Lyngby, Denmark

**G. Limbert **

National Centre for Advanced Tribology at Southampton (nCATS) | Bioengineering Science Research Group, Faculty of Engineering and the Environment, University of Southampton, Southampton SO17 1BJ, UK; Biomechanics and

Mechanobiology Laboratory, Biomedical Engineering Division, Department of Human Biology, Faculty of Health Sciences, University of Cape Town, Anzio Road, Observatory 7925, South Africa

**J.F. Molinari and G. Anciaux **

LSMS, ENAC, Swiss Federal Institute of Technology (EPFL), CH-1015, Lausanne, Switzerland

**R. Aghababaei**

Department of Engineering, Aarhus University, Inge Lehmanns Gade 10, 8000 Aarhus C, Denmark

**S. Echeverri Restrepo **

SKF Engineering & Research Centre (ERC), SKF B.V., Nieuwegein, the Netherlands; Department of Physics, King's College London, Strand, London WC2R 2LS, England, UK

**A. Papangelo **

Hamburg University of Technology, Department of Mechanical Engineering, Am Schwarzenberg-Campus 1, 21073 Hamburg, Germany

**A. Cammarata and P. Nicolini **

Department of Control Engineering, Faculty of Electrical Engineering ,Czech Technical University in Prague, Karlovo namesti 13, 12135, Prague 2, Czech Republic

**C. Putignano, G. Carbone and M. Ciavarella **
Politecnico di Bari. V. le Gentile 182, 70125 Bari-Italy

**S. Stupkiewicz and J. Lengiewicz **

Institute of Fundamental Technological Research, Polish Academy of Sciences, Pawinskiego 5B, 02-106 Warsaw, Poland

**G. Costagliola****and F. Bosia **

Department of Physics and Nanostructured Interfaces and Surfaces Centre, University of Torino, Via Pietro Giuria 1, 10125 Torino, Italy

**R. Guarino **

Laboratory of Bio-Inspired & Graphene Nanomechanics, Department of Civil, Environmental and Mechanical Engineering, University of Trento, Via Mesiano 77, 38123 Trento, Italy

**N.M. Pugno **

Laboratory of Bio-Inspired & Graphene Nanomechanics, Department of Civil, Environmental and Mechanical Engineering, University of Trento, Via Mesiano 77, 38123 Trento, Italy; Ket Lab, Edoardo Amaldi Foundation, Italian Space Agency, Via del Politecnico snc, 00133 Rome, Italy;

School of Engineering and Materials Science, Queen Mary University of London, Mile End Road, E1-4NS London, United Kingdom

**M.H. Müser **

Department of Materials Science and Engineering, Saarland University, 66123 Saarbrücken, Germany

* Corresponding author. E-mail: mciava@poliba.it

2
**Abstract **

This review summarizes recent advances in the area of tribology based on the outcome of a Lorentz Center workshop surveying various physical, chemical and mechanical phenomena across scales.

Among the main themes discussed were those of rough surface representations, the breakdown of continuum theories at the nano- and micro-scales, as well as multiscale and multiphysics aspects for analytical and computational models relevant to applications spanning a variety of sectors, from automotive to biotribology and nanotechnology. Significant effort is still required to account for complementary nonlinear effects of plasticity, adhesion, friction, wear, lubrication and surface chemistry in tribological models. For each topic, we propose some research directions.

**Keywords: tribology, multiscale modeling, multiphysics modeling, roughness, contact, friction, **
adhesion, wear, lubrication, tribochemistry

**1. Introduction **

The word tribology introduced in the famous Jost report of 1966 [1] was apparently coined by David Tabor and Peter Jost, deriving from the root tribo- (Greek τρίβος, meaning “rubbing”) and the suffix - logy (Greek -λογία, meaning “the study of”). The Jost report suggested that problems of lubrication in engineering needed an interdisciplinary approach –including chemistry and materials science, solid mechanics and physics. At that time, Jost suggested that the British industry could have saved £500 million a year “as a result of fewer breakdowns causing lost production; lower energy consumption;

reduced maintenance costs; and longer machine life.” Fifty years later, frictional losses are often evaluated as costing more than 1 per cent of GDP [2], and tribology is therefore still flourishing.

There is no doubt that tribological interactions have a profound impact on many areas of engineering and everyday life. The widespread significance of these effects has been highlighted in many articles and reports over the years, which, until recently have mainly focused on lubrication and friction and wear-related energy and material losses for “traditional” industrial applications, such as manufacturing and automotive. The reader is referred to recent reviews, which have, for example, looked at the development of solid lubricant coatings [3], lubrication [4], and the interplay between surfaces and lubricants [5]. Other works have focused on how improvements in friction reduction technologies could significantly reduce frictional energy losses in passenger cars in the short, medium and long term [6]. Reducing wear can also improve long-term efficiency and performance of moving components, as well as reducing costs of maintenance and/or improving quality of life. Accordingly, much research into means of reducing friction and wear, together with the development of new additives, lubricants and functional materials to improve the performance of interfaces, has taken place, typically in the form of experimental studies for developing improved surface materials, topography/textures or lubrication. Most of these activities have been supported and accompanied by fundamental developments in contact mechanics, e.g. [7,8], as well as surface and material science, e.g., [9]. This has in turn improved our understanding of how surface roughness and surface modifications affect the response of components in various applications [10,11].

More recently, new areas of tribology have emerged, including nanotribology, i.e. the study of friction, wear and lubrication at the nanoscale as applied, for example, to micro- and nano-electromechanical systems (MEMS/NEMS), e.g., [12,13], and magnetic storage, e.g., [14,15], and biotribology, which deals with human joint prosthetics, dental materials, skin, etc., and ecological aspects of friction, lubrication and wear (tribology of clean energy sources, green lubricants, biomimetic tribology) [2,16- 19]. Studies of superlubricity, i.e. the mechanisms responsible for extremely low friction [20-23], have created great expectations of energy savings, and the creation of graphene is also greatly promising in

3

this direction [24]. Insects' and reptile's adhesive performance inspired numerous studies on adhesive contacts (e.g. [25-29]) and resulted in improved understanding and successful mimicking of Nature- made feet [30-37]. Massive usage of tactile interfaces triggered multiple studies in understanding sensing through contact and friction [38], and in reproducing interactive haptic feedback to moving fingers [39-42]. In keeping up with and enabling such developments, new knowledge is necessary to describe complex multiscale and multiphysical phenomena within the context of tribology, both in the modeling and experimental domains.

In this contribution, we aim to summarize the presentations and discussions that took place during a Lorentz workshop on “Micro/Nanoscale Models for Tribology” in Leiden, the Netherlands, between 30 January and 3 February 2017. It was found that one of the key issues facing the tribology community is the apparent disparity between the fields of expertise relevant to such an interdisciplinary topic, which leads to a lack of communication between engineers, material scientists, applied physicists and chemists who work to solve similar tribological problems: differences exist in notation, language, methods, the way in which problems are posed and how solutions are presented.

Another finding is that new analytical models are necessary to understand the behavior at tribological interfaces, partly to avoid that numerical simulations become “black boxes” where the nuances of the phenomena involved are lost, and partly because full computational models often require prohibitively long computational times. At the same time, the industry would benefit from lightweight analytical models as long as those are sufficiently robust and able to predict critical quantities of interest with a priori known precision. Further adding to these challenges is the complexity of model validation: as the contact interface in most cases is not accessible to direct in situ observations, it is very difficult to carry out experiments aiming to access local near-surface states.

Difficulties are further enhanced by divisions between modelers and experimentalists, as well as those working on analytical versus computational methods –and also between the proponents and users of different theories, computational methods and tools– and depending on the research applications.

Since increased visibility and cooperation between tribologists from different backgrounds is necessary, the present review aims at providing a starting point for further collaboration and possible focal points for future interdisciplinary research in tribology. Accordingly, the paper is organized as follows: various modeling methods and tools are discussed in §2; research themes in tribology, including multiphysical aspects, rough surface representations, scale effects and the breakdown of continuum theories at the nano- and microscales, material models, normal contact, friction and other phenomena, as well as interdisciplinary case studies in biotribology are addressed in §3, and conclusions are given in §4.

**2. Tribological modeling methods **

This section introduces the main tools currently used in tribological modeling, starting from analytical models and discussing continuous and discrete mechanical and multiphysical methods suitable for simulations characterized by different time- and length-scales (see Fig. 1 for a map of representative tribological models built across the scales), namely finite and boundary element methods, discrete dislocation dynamics and atomistic methods, as well as multiscale approaches.

4

Fig. 1: A time- vs. length-scales map of models developed in tribology highlighting the intrinsic link between multiscale/physics that needs to be captured to provide predictive tools for engineering applications. Illustrations from simulations performed by the authors.

**2.1. Analytical Methods **

**2.1.1. Contact mechanics: where we stand **

A full overview of the field of contact mechanics and related developments that took place over the last century or so is out of the scope of the current contribution, as this would require a devoted review. For someone approaching this scientific area for the first time, K.L. Johnson's Contact Mechanics book [43] is still a very good starting point today. Later books and review papers, e.g. [44- 49], have accounted for some of the progress made, but the field continues to expand across disciplines. The purpose of this sub-section is to briefly summarize some of the important milestones in this field and provide pointers to the readers interested in its different branches.

Starting from the mechanics of nominally smooth contact problems, the Hertzian theory, which solves the problem of two non-conformal elastic bodies being subjected to frictionless contact [50], is considered as a cornerstone of contact mechanics and tribology. Many of the analytical solutions available to practitioners and scientists have been building on Hertz; as is the case, for example, for two early models that constitute seminal advances in contact mechanics focused on the issue of adhesion: the models by Johnson-Kendall-Roberts (JKR) [51] and Derjaguin-Muller-Toporov (DMT) [52]. While the JKR and DMT models, which describe the adhesive contact between compliant or hard spheres, are still very popular, the body of literature available on this topic is very substantial, especially given its relevance to, e.g., biomimetic applications; adhesion is discussed in detail in §3.7.

Remaining in the realm of smooth contact problems, but moving away from the Hertzian theory of elastic contacting bodies and its limitations (only accurate for small contact areas), progress has been made in a number of other areas: these include, for example, layered and coated systems, also in the presence of anisotropic and functionally graded materials [53-61], contacts in the presence of sharp edges [62-65] and conformal configurations [66]. Other examples of recent developments in the field are the use of asymptotic analyses to study the stress fields and sliding behavior associated with different contact configurations [67-70], the study of contact in the presence of anisotropic and

5

functionally graded materials, and varying friction coefficient along the interface in sliding and partial slip conditions [71]. In the case of the normal contact of inelastic solids, significant developments have been made since Johnson’s core model of elasto-plastic indentation based, for example, on the progress of instrumented nanoindentation in the last 25 years (see, e.g., [72-74]); issues of plasticity and material models are discussed further in §3.4. Some progress has also been made on tangential loading and cyclic contact with the generalized solution of contact problems characterized by time- dependent stick-slip transitions at the macroscopic scale (see, e.g. [62,75-79]).

Somewhat in parallel to the above advances and studies, many developments in the study of nominally smooth contacts in the presence of lubrication have also been made; these are discussed in §2.4 and

§3.8.

On dynamic effects and impact, much work was published on the rate-and-state friction (RSF) law (also discussed in §3.6.2) and Adams’ instability [80-82], while impact remains a somewhat separate and large research area, with applications in different research area and applications including powder technology, manufacturing processes and ballistics [83-88]. Following the classical contributions by J.R. Barber on both static and sliding contact reviewed in Johnson’s book, new refined solutions and finite element formulations have appeared on thermoelastic contact (see, e.g., recent contributions [89,90] and further discussion in §2.6).

Moving on to applications strongly linked to the development of contact mechanics methodologies, various advances have been made. An example is the development of various techniques used to individually or simultaneously study various aspects of fretting fatigue, such as stress gradients, fatigue, surface damage and wear [91-96]. Progress has also been made in the study of rolling contact of elastic and inelastic (shakedown, ratchetting, etc.) bodies and rolling contact fatigue (see, e.g., [97- 104]). Calendering, i.e. the elastic-plastic rolling of strips have also seen some developments [105].

On the topic of contact mechanics of rough surfaces, the seminal work by Greenwood and Williamson (GW) [7] forms the basis for a number of multi-asperity models (discussed critically in §2.1.2).

Among many subsequent analytical models, some were developed based on the analysis of two or more scales, adding for example the periodic microgeometry of multi-layered elastic or viscoelastic half spaces to study normal contact and friction in the presence of coatings [106,107] or adhesion and lubrication [108,109]. Interestingly, one of the most popular theories after the GW is that of Majumdar and Bhushan [110], where Korcak’s law was used to define a power law distribution of contact spots, a “bearing area” result very much in contrast with the present understanding of the contact area being formed by “resolution-dependent” contact spot sizes. This view of “magnification-dependent” solution is not too different from the original Archard model [111] of spheres sitting on top of spheres, or work on fractal description based on a Weierstrass series within the elasticity assumption to obtain the result that the contact area decreases without limit as the resolution (or magnification) is increased [112].

The alternative to the solutions proposed in the methodologies to study rough contacts reviewed above is Persson’s theory [8], which has become the basis of another class of models, in which the stress probability distribution is considered as a function of the surface resolution under examination. The tribology community still uses both the GW and Persson approaches to model rough contact based on considerations of accuracy and simplicity which may well reflect the corresponding physics and engineering perspectives. The GW and Persson models are introduced in more detail next; a comparison between them in the context of the recent contact-mechanics challenge [113] is given in

§3.5, while the topic of roughness itself is described extensively in §3.2.

6

**2.1.2. Multi-asperity models and Persson’s theory: an introduction **

The nature and various representations of surface roughness, discussed in more detail in §3.2, have been central to the prediction of tribological quantities ranging from the true area of contact –in contrast to the apparent or effective area– to the normal, friction and adhesion forces, as well as phenomena such as electrical conductance and percolation. Starting from the simplest problem definition of normal contact between two rough surfaces in the absence of other phenomena, two seminal works have formed the backbone of research in the field: the Greenwood-Williamson (GW) model [7] and Persson’s theory [8]. These are introduced below, while the results of a recent contact- mechanics challenge are summarized in §3.5, extending beyond predictions of the true contact area and into more detailed metrics of normal contact.

Greenwood and Williamson conducted a pioneering study targeted towards predicting the link between the approach of nominally flat but rough surfaces (quantified as the distance between their mean planes) and the resulting force and true contact area [7]. The GW and subsequent multi-asperity models are based on the following assumptions: 1) the effective rough surface (a superposition of two rough profiles or surfaces) can be represented by an ensemble of asperities (surface summits), characterized by the vertical coordinate of the tip and its curvature(s); 2) these characteristics are known in the statistical sense, for example, via the probability density of the asperities' vertical position; 3) the relation between penetration, force and the contact area follows the Hertzian theory of contact; 4) the asperities of the effective rough surfaces coming into contact are separated in the plane by distances at which their mutual influence can be neglected. In the original GW, all asperities are approximated as parabolic with the same curvature radius, and an arbitrary height distribution is assumed, contrary to numerous references in the literature erroneously stating that the GW model is based on Gaussian distribution of asperity heights: both Gaussian and exponential tails are considered in the original paper.

Subsequent progress in statistical multi-asperity models was triggered by the seminal paper of Nayak
[114], which was in turn inspired by the works of Longuet-Higgins who was the first to apply the
random process model for analysis of random surfaces in the ocean [115,116]. Based on the same
assumption, i.e. that a rough surface can be represented as a two-dimensional isotropic Gaussian
process, Nayak obtained the relation between the spectral moments of the surface and the distribution
of asperities, their density, curvature, ellipticity, etc. He also introduced a central quantity for
roughness description, a dimensionless combination of the zeroth, second and fourth momenta,
*subsequently referred to as the Nayak parameter that characterizes spectral breadth. Based on Nayak's *
statistical results, Bush, Gibson and Thomas (BGT) [117] obtained a new approximation for the
dependence of the force density and contact area fraction taking into account, among other of Nayak's
results, the ellipticity of asperity tips. Much later, Greenwood [118] demonstrated that, according to
Nayak's theory, the ellipticity of asperities is rather mild, and thus an approximate Hertzian equation
for the elliptic contact can be employed, which makes use of the geometric mean value of two
principal asperity curvatures. This “simplified elliptic model” yields relatively simple equations for
force and area dependence as functions of the approach (or separation). Among other interesting
results, Greenwood demonstrated that according to the random process model, the probability of
finding a spherical asperity is strictly zero.

Multi-asperity models predict asymptotic linearity between the contact area and the load with a factor containing a proportionality coefficient 𝜅 and, in the denominator, a product of the effective elastic modulus and the root mean squared roughness gradient (or equivalently, a square root of the doubled second spectral moment). However, it is important to remark here that this proportionality holds only for vanishingly small contact area intervals, which depend on the Nayak parameter: the higher this

7

parameter is, the smaller the region of validity [118-120]. In this light, the proportionality predicted between the load and the area remains a mathematical abstraction and cannot be used directly in engineering practice. However, the usage of multi-asperity models is not restricted to vanishingly small areas, but can also be used for higher loads at which the area evolves nonlinearly with the load and strongly depends again on the Nayak parameter [117,120]: the higher the Nayak parameter, the smaller the contact area. Comparison of multi-asperity models with full numerical simulations of rough contact (free of the multiple assumptions of multi-asperity models) demonstrated that, indeed, the Nayak parameter plays an important role in contact area evolution, but its effect in multi-asperity models is strongly exaggerated [121].

Further improvements in multi-asperity models attempted to incorporate elastic interaction between asperities, based on the following motivation: if one asperity comes into contact and produces a force, then the vertical position of all surrounding asperities needs to be changed by, approximately, a value proportional to this force and inversely proportional to the distance to its point of application (for the precise formulations refer to [43]). Note that because of such a slow decay, this long-range elastic interaction cannot be cutoff without considerable loss in accuracy. Approximately, this interaction can be included in a statistical framework by assuming a zero-order approximation, i.e. the vertical positions of all asperities are decreased by a value proportional to the product of a nominal pressure and the contact area [122-124]. A further improvement in terms of elastic interaction relied on the rejection of a purely statistical model and the resorting to deterministic models instead, taking into account the in-plane positions of all asperities. In this deterministic framework, not only elastic interactions can be accurately accounted for [119,125], but so can the merging of contact areas related to distinct close asperities [126].

In 2001, B.N.J. Persson suggested another analytical model for predicting the contact area and other related quantities [8] that relies on completely different considerations and, therefore, does not suffer from the multiple assumptions inherent in multi-asperity models (even though it introduces its own).

Persson’s theory is based on the following consideration: let us assume contact between two flat
surfaces squeezed together by a nominal pressure 𝑝_{0} such that the probability density of interfacial
pressure is simply a Dirac delta-function centered at 𝑝_{0}. When new modes are progressively injected
into the spectrum of contacting surfaces, the corresponding pressure distribution function spreads out
as a Gaussian distribution. If the full contact is preserved, the link between the statistical
characteristics of the height distribution and interfacial pressure distribution can be easily established:

the variance of the contact pressure is proportional to the product of the variance of the surface gradient and squared effective elastic modulus. Based on these considerations, a diffusion-type equation was formulated for the contact pressure distribution (acting as the concentration quantity), with the pressure variance acting as the time and the local pressure acting as the space coordinates [8,127,128] considering, up to this point, only full contact. Since Gaussian support is infinite, tensile stresses will occur in the contact interface for an arbitrary finite external pressure. To get rid of these and extend the theory to partial contact, Persson introduced a boundary condition stating that the probability density of zero pressure vanishes during contact. This statement can be confusing since, as soon as partial contact is established, all non-contact zones do not experience any contact pressure, thus resulting in Dirac-delta function distributions at zero pressure scaled by a factor of the non- contact area fraction. Alternatively, this boundary condition can be stated in a limit-form: probability density tends to zero as pressure tends to zero. Indeed, this boundary condition seems very reasonable if one thinks about the fact that, for Hertzian contact, the pressure drops to zero at the contact edges with an infinite slope, thus resulting in the linear growth of probability density near zero pressure. The

8

main remaining assumption of Persson's theory is the validity of the diffusion equation for partial contact accounting for the fact that it was derived for full contact.

Apart from other quantities of interest, Persson's theory predicts that the contact area evolves as an error function, from zero to full contact, which is reached for infinite nominal pressure. Since the Taylor expansion of the error function in the vicinity of zero contains only odd powers, the contact area can be approximated with a high degree of confidence by a linear function of nominal pressure with a factor given by a proportionality coefficient divided by the product of a root mean squared roughness gradient and the effective elastic modulus. The first difference between this prediction and those of multi-asperity models is the proportionality factor 𝜅, which is approximately 1.60 in Persson's theory and approximately 2.51 in multi-asperity models. The second crucial difference is that, contrary to multi-asperity models, Persson's linearity is valid for realistic area/pressure intervals. Finally, the third difference is that the sole roughness parameter needed for Persson's theory is the root mean squared roughness gradient so that, contrary to multi-asperity models, this theory has no dependence on the Nayak parameter.

Numerous comparisons between complete numerical simulations, multi-asperity models and Persson's theory can be found in the literature [119-121,127-141]. The rough conclusion of all these studies with respect to the contact area evolution can be formulated as follows: Persson's model nicely predicts the qualitative growth of the contact area with increasing nominal pressure up to full contact. For moderate loads, the true contact area evolves slightly nonlinearly and is below the asymptotic prediction of multi-asperity models and above the prediction of Persson's theory. On the other hand, Persson's theory accurately predicts the contact area near full contact [137]. Meanwhile, an improvement in Persson's theory was introduced to take into account partial contacts in a more rigorous way [142], yielding results that are much closer to numerical solutions. Very recent findings demonstrate that the contact area growth is dependent not only on the root mean squared gradient but also weakly on the Nayak parameter [121] which is absent in Persson's theory, but is inherent to multi- asperity models that, however, strongly overestimate its effect.

**2.2. Finite and Boundary Element Methods **

Two major families of methods can be distinguished in continuum mechanics: the Finite Element Method (FEM) [143] and the Boundary Element Method (BEM) [144]. The FEM is a versatile method for solving boundary value problems in many fields of science and technology [143,145,146]).

In the FEM, an explicit relation between the strain (and possibly strain rate and its history) and the stress can be prescribed, either within infinitesimal or finite strain formulations, enabling this method to consider arbitrary constitutive material models starting from simple linear elasticity up to complex crystal plasticity. The BEM uses in its formulation a fundamental solution for the normal and tangential point forces, which enables linking surface tractions with surface displacements.

Equivalently, to formulate a spectral version of the BEM, a fundamental solution linking pressure and vertical displacement for a combination of harmonics in two orthogonal directions should be used [147,148]. Such solutions exist for a limited number of cases and mainly under the assumption that the solid can be locally considered as a flat half-space. These limitations imply a more restrictive field of application for the BEM compared to the FEM, which is a versatile numerical method. It is worth mentioning that, in general, contact problems are nonlinear even if frictionless and non-adhesive contact is considered between linearly elastic solids. This is because the contact area is a priori unknown, apart from simple cases such as the rigid flat stamp problem or the case of full contact. In analogy, a full stick frictional condition (infinite friction) makes the frictional problem much easier to handle than a problem with a finite friction.

9

Detailed descriptions of numerical methods within the FEM formulation can be found in the literature, e.g., [149-151], while details on the application of the BEM in rough surface contact mechanics can be found in a comparative analysis of BEM formulations [152]. There are also many instances in which FEM and BEM can be coupled into FEM-BEM solvers for the solution of three-dimensional contact problems [153] or can be combined to achieve different levels of refinement in the solution to the problem under investigation (see, e.g., [154]).

The application of the FEM to tribological problems involves the discretization of the volumes of contacting bodies and an appropriate treatment of their contact interaction. The arbitrariness of material models, as well as the geometries of contacting solids and their heterogeneity that can be reached in the treatment of contact interfaces, make this method a multipurpose engineering tool.

However, this is all at the cost of a higher computational complexity than in the BEM, which has less versatility but a much higher efficiency in the treatment of interfacial problems, since it requires solving the problem only for surface degrees of freedom and does not require any discretization in the volume. On the other hand, the BEM results in dense systems of linear algebraic equations, contrary to the FEM, which renders sparse systems of equations. Thus, the BEM has to rely on iterative solvers, whereas the FEM can successfully use either iterative or direct solvers based on the sparse matrix storage.

When interested in near-surface stress fields, which are crucial in the reliable analysis of surface deterioration (e.g., fretting fatigue and wear) and microscopic contact at the roughness scale, imprecise integration and/or discretization may result in huge errors in local fields and, thus, in realistic estimations. To properly capture the stress field in the vicinity of a contact zone, and especially near its edges (which, in most problems, is unknown), requires a very dense spatial discretization. The accuracy of the integration technique is especially crucial when a conformal mesh cannot be ensured on the contacting parts (e.g., large-deformation or large-sliding contact systems) and if two deformable solids of comparable stiffness are brought into contact, i.e., when one of the solids cannot be considered as rigid. In addition, the path-dependence of frictional problems requires that the load increment should be chosen properly, as the temporal discretization plays a crucial role even in quasi- static problems: as an example, for the shear tractions in normal Hertzian cylindrical contact with friction in the interface, the self-similar character of the solution, as argued by Spence [155], can be obtained with one hundred load steps with the displacement increment proportional to the time squared, but not within one single load step.

In tribology, due to its computational cost, application of the FEM is justified if the problem at hand cannot be solved within the assumptions of the BEM, namely the existence of a fundamental solution and the local flatness of the surface (small slope). A broad family of systems falls within this context:

large-deformation, large-sliding contact of soft bodies, which can be observed in various biological systems (oral food processing, contact of skin, etc.), but also in engineering applications (contact of tires, polymeric seals and many others) or contacts involving strongly nonlinear material behavior which is hard to represent within the BEM framework such as indentation involving strong finite- strain plastic deformations or fracture in the interface.

Concerning the applications to microcontacts and microtribology, both FE and BE methods are used extensively. At the scale of roughness, the macroscopic shape of the contacting solids can be usually neglected and, since the roughness slope is in general rather small, the problem satisfies the main assumption of the BEM, which can be successfully used for its solution. The evolution of the true contact area, interface permeability, electric and thermal contact resistance can all be resolved in the framework of the BEM for linear material laws. Regarding material nonlinearities, elasto-plastic [156-

10

158] and viscoelastic [159,160] material behavior can be incorporated in the BEM framework by assuming that deformations and slopes remain small, otherwise an FEM would be needed [161,162]. It should remarked that most contact systems involving elasto-plastic materials operate mainly in the elastic regime both at the micro- and macroscales; hence, depending on the level of stress and the type of loading, considering plastic deformation may be important during the first loading cycles but may not be needed in subsequent ones. Furthermore, severe plasticity is associated with wear and must therefore be incorporated in the simulations, but how can one explicitly model wear numerically (e.g.

using both BEM and FEM)? The issue of wear is partly discussed in §3.9.1.

The BEM framework can consider homogeneous nonlinear material behavior, but can also account for heterogeneous inclusions in the bulk, see e.g., [163], which is computationally much more expensive.

Accounting for heterogeneous materials is often critical for microscale analyses in which the material’s microstructure might play an important role. This, for example, is the case in contact problems involving functionally graded interfaces [164], metallic polycrystalline [165] or monocrystalline [166] microstructures, whose accurate treatment requires the FEM. Concerning multiphysical (multi-field) problems, both methods are comparable at the scale of roughness, with the same limitations and advantages: simple but fast BEM versus slow FEM but with capabilities to account for arbitrary complexity. Examples of applications include: lubrication problems [167-169], electro-elastic contact modeling [170,171], thermo-mechanical coupling [172], and many others.

Using BEM-type formulations has also been used to treat elasto-dynamic frictional problems [173,174], whereas complex geometries and boundary conditions would still require usage of FEM or equivalent formulations [175,176].

In summary, both the FE and BE methods are well developed and able to solve most micro- tribological problems involving both material nonlinearities and multiphysical couplings with the FEM being more versatile and more easily accessible for a general researcher and engineer (numerous commercial and open software are available) but computationally costly, and the BEM being less available and versatile, but still capable of solving most problems under reasonable assumptions and for very moderate computational costs. The main challenge here for the researchers and engineers would be to promote both methods within the homologue communities and to enable them to use one or the other based on the needs of the target application.

**2.3. Crystal plasticity and Discrete Dislocation Dynamics **

Crystal plasticity is a well-established constitutive framework for the modeling of elasto-plastic deformations of metal crystals [177-180]. The essential feature of crystal plasticity is that plastic deformation is assumed to result from plastic slip on specified crystallographic slip systems. An individual slip system is active when the shear stress acting on it (called the resolved shear stress) exceeds the corresponding critical resolved shear stress, the latter being governed by an evolution (hardening) law that is expressed in terms of slip rates for all active slip systems. By considering the crystallographic features of plastic deformation, crystal plasticity provides a physics-based continuum description of single crystals as well as of individual grains in polycrystalline aggregates [181,182].

Once combined with a suitable scale transition scheme (mean-field homogenization, Representative Volume Element (RVE)-based computational homogenization, etc.), crystal plasticity has proven to be highly successful in predicting the effective elasto-plastic behavior of polycrystalline aggregates, e.g., [183-185]. A notable example is the visco-plastic self-consistent (VPSC) model [186], which is widely used for predicting hardening and texture evolution in plastic forming processes. The crystal plasticity framework has also been extended to include, in a simplified manner, other deformation mechanisms, such as deformation twinning [187,188] and martensitic phase transformations [189,190].

11

Being a continuum theory, crystal plasticity is not applicable at very small scales at which discrete events, e.g., those related to the nucleation and propagation of dislocations, become important, and other approaches, such as discrete dislocation dynamics (see below) and molecular dynamics (see

§2.4), are then more appropriate. Even at higher scales, important phenomena that accompany plastic deformation, e.g., the formation of dislocation structures, deformation banding and grain refinement, are not captured by the available crystal plasticity models, even though attempts in that direction have been made [191-194]. In general, plastic deformation is inhomogeneous at multiple scales, and crystal plasticity is not capable of describing many of the related phenomena.

Discrete Dislocation Dynamics (DDD) is a modeling technique to study plasticity at the microscale [195-200]. In DDD, the solid is modelled as a linear elastic continuum, and the dislocations by means of their linear elastic fields, which are accurate outside of the dislocation core. Atomistic aspects are included by means of constitutive rules that govern dislocation nucleation/annihilation, glide, and interaction with obstacles and dislocations. Given that both the dislocations and the solid are described using linear elasticity, it is possible to solve boundary value problems relying on the principle of superposition. The solution to the boundary value problem is given at each time increment and at every material point as the sum of the dislocation fields and their image fields. The image fields can be calculated using finite elements, although, for contact problems, where rough surfaces need to be described using a fine discretization, it is computationally more efficient to use other techniques, such as, for instance, Green’s Function Molecular Dynamics (GFMD) [201].

Important recent advances in this area include, for example, the development of a formulation that incorporates elastodynamic effects in the description of the interactions between dislocations. The resulting methodology, Dynamic Discrete Dislocation Plasticity (D3P; see, e.g., [202]), allows the treatment of problems characterized by high strain rate deformation such as shock waves [203] and could be used to perform concurrent coupling (see §2.6) with atomistic simulations in order to avoid issues with the transition between the atomistic-continuum boundaries. Furthermore, concurrent methodologies (also see §2.6) to directly couple crystal plasticity and DDD have been also developed [204,205] to take advantage of the fact that the DDD formulation is only required in very small regions in the presence of stress concentrations, such as cracks and indentation of asperity-to-asperity interactions.

**2.4. Modelling Methods for Lubrication, Solid/Fluid Interactions and Particle Dynamics **

The computational methods introduced in the previous two sections mainly cover formulations and methodologies adopted to model individual dry contact problems and focus on detailed descriptions of solid deformations and stresses. However, other techniques must be adopted when modelling lubrication and solid/fluid interactions in the presence of a fluid film interposed between contacting bodies and when multiple contacts are generated simultaneously through the complex interactions between many particles. In this sub-section, we give an overview of standard and advanced methods developed over the last century to predict film thickness, friction, rheological response of fluids and interactions between surfaces in lubricated conditions. A brief summary of the techniques developed to study interactions between particles in different environments and the dynamics of systems involving multiple contacts is then provided.

Hydrodynamic Lubrication (HL) and Elasto-Hydrodynamic Lubrication (EHL) are lubrication regimes where a thin lubricant film is formed between two surfaces in relative motion. HL takes place in conformal contacts, when low pressures are established between the two surfaces, while EHL takes place when pressures are significant enough to cause considerable elastic deformation of the surfaces.

EHL usually occurs in non-conformal contacts and many machine elements, including rolling bearings

12

and gears, rely on EHL in their operation. Existence of a fluid film sufficient to separate two surfaces under hydrodynamic conditions, such as in a journal bearing, has been known since the work of Tower in 1883 [206]; however, it was not until 1949 that Grubin predicted that a thin fluid film can also separate surfaces in high pressure, non-conformal contacts [207]. Formation of such a film is possible due to high pressure having two beneficial effects: firstly, it increases lubricant viscosity in the contact inlet and, secondly, it elastically deforms and flattens the contacting surfaces, hence the term elasto- hydrodynamic lubrication.

Classical solutions of HL and EHL contact problems use the Reynolds’ equation [208] to describe the behavior of the lubricant, while elastic deformation is traditionally calculated using Hertz theory of elastic contact, although nowadays BEM or FEM solvers are also routinely used. Reynolds's equation is a simplification of full Navier-Stokes equations, derived by assuming a Newtonian lubricant with constant density and constant pressure and viscosity across the film thickness. Cameron et al. [209]

developed the first Reynolds-based computerized numerical solutions for hydrodynamic lubrication and in 1959 Dowson and Higginson [210] produced the first full numerical solution for EHL.

Subsequently, Dowson and co-workers, also proposed regression equations for prediction of the EHL film thickness based on their numerical solutions and a number of other improvements including the consideration of material properties and thermal effects (e.g., [211-213]. In the last fifty years, many numerical approaches [214-218] have been developed to address the solution of this set of equations:

nowadays, it is possible to account for a variety of non-Newtonian effects, ranging from piezo- viscosity to shear thinning. The majority of these approaches uses a Finite Difference (FD) scheme, although the use of the FEM and Finite Volume (FV) methodologies has recently been proposed especially to overcome some of the limitations of FD when dealing with complex domains in the presence of micro-textured surfaces and cavitation using mass-conserving algorithms [219-221], but also to extend a Reynolds-type solver to full Computational Fluid Dynamics (CFD) studies looking at the fluid flow outside the contact, overcoming the limitations of the Reynolds’ assumptions in specific extreme contact conditions [222-225]. The development of fully-coupled Solid/Fluid Interactions (SFI) solvers [226] constitutes the new frontier of this particular area of research, with the promise that advances in computational power may lead to a more comprehensive study of the multiphysics phenomena governing three-dimensional contact problems considering full field deformations, thermal and multi-field effect, and the complex rheologies of the fluids and the solids under investigation.

Hybrid techniques (e.g., the element-based finite volume method – EbFVM [227,228]) have also been recently developed to combine the flexibility of finite elements in terms of studying complex domains and using unstructured meshes and the use of finite volumes to accurately solve the fluid-dynamic problem at hand.

Another important area of interest, often to industrial applications, is the solution of problems involving particle interactions and multi-body contacts, as many industrial and natural processes involve granular systems. Diverse phenomena such as avalanches, fluidized beds and asthma inhalers all depend on assemblies of particles. The understanding of such systems is therefore of interest to a number of scientific disciplines, as well as industry. Due to their complexity, it is often very difficult to study such systems, in which large numbers of particles interact, and macroscopic behavior depends both on the physical properties of individual particles, and the interactions between them. The Discrete Element Method (DEM) is ideally placed to tackle these contact configurations, as it allows the description of the physical state of a system using a large number of discrete elements. This approach shares many similarities with atomistic simulations (see §2.5) where atoms are replaced by particles that interact via constitutive equations rather than interaction potentials; however, depending on the problem under investigation, the DEM requires constitutive laws to describe individual interactions,

13

which often are obtained by adopting hierarchical multi-scale approaches (see §2.6). Noticeable examples are studies of particle-particle interactions to derive elastic, viscoelastic and plastic constitutive laws that capture the right kinematics during particle collisions [229-232] and the integration of the effect of adhesion [233,234], particle shape [235,236] and roughness [237,238] into DEM codes. Recently this method has been also used to study wear involving complex fragmentation, but also problems affected by complex rheological and/or multi-physics behavior [239,240].

**2.5. Atomistic methods **

Molecular Dynamics (MD) was first developed to study the interaction of hard spheres [241] and, in the following decades, has been expanded into methods and tools suitable for investigations in a number of physical, chemical and mechanical phenomena both for diagnostic [242-247] and predictive purposes [248-257]. Classical MD essentially calculates the kinematics of atoms (or representative

“particles”) by solving their Newtonian (or Langevin) equations of motion based on potentials that describe the interactions between them. This tool was applied to the study of tribological interfaces especially in the high speed regime, which lends itself to the length and timescales of MD [258-261].

Other examples of studies include: elementary phenomena such as the mechanical mixing between two surfaces in contact [262]; different wear regimes [263], plastic deformation [264,265]; the tribology of Diamond-Like Carbon (DLC) coatings [266]; the frictional behavior of self-assembled layers formed from additives [267,268]; the rheology of lubricant films in contact in the EHL regime [269,270]; and other tribological phenomena including friction, adhesion, and wear [271].

The classical MD framework can provide a description of the dynamics at atomistic level, but without
explicitly modelling individual interactions in terms of surface reactivity, bond formation and
*evolution of electronic structures, which can be dealt with using first principles or ab initio MD *
techniques (examples of this include Car-Parrinello MD [272] and Tight-Binding Quantum Chemical
MD (TB-QCMD) [273] and will be discussed in more detail at the end of this sub-section); hence, the
key ingredient of any classical MD simulation is the interaction potential (also referred to as the Force
Field, FF). Even though the availability of suitable interaction potentials is still a limiting factor for the
study of complex systems, several families of FFs have been presented in the literature (along with
their explicit parameterization), each of them designed to capture the essential features of a different
type of material. The simpler functional forms of FF are represented by pairwise interactions that
generally account for an attractive (describing London dispersion forces) and a repulsive term
(originating from core-core repulsion). Probably the most popular examples are the Lennard-Jones
(LJ) [274] and Morse potentials [275]. The number of (free) empirical parameters is kept at a
minimum (for each atomic species, this number is two and three for the LJ and Morse potentials,
respectively), as is the computational cost of simulations based on these FFs. It turns out that the LJ
and Morse potentials are not able to realistically describe the behavior of many materials (for example,
the LJ potential can accurately model noble gases only). Nevertheless, the usage of the LJ potential
has produced fundamental results over the years, as evinced, for example, in the prediction of the
breakdown of continuum contact mechanics at the nanoscale [276,277], discussed in more detail in

§3.3, and in Non-Equilibrium MD (NEMD) simulations to shed light on the phase behavior of fluids in confinement [278-280].

Metallic systems are more often (and more accurately) described by the family of the Embedded Atom Method (EAM) potentials [281]. EAM potentials comprise a pairwise repulsive term modeling the core-core interaction and a cohesive contribution representing the energy that an ion core experiences when it is “embedded” in the electron density originating from neighboring atoms. The use of these many-body potentials overcomes intrinsic limitations of two-body potentials, which, for example, are bound to satisfy the Cauchy relation, or lead to defect energies that correlate with cohesion energies

14

much more strongly than in real materials.. Examples of the application of the aforementioned potentials in tribology are studies of the frictional behavior of an indenter tip against different metallic surfaces [282-285], or the interfacial friction characteristics of different metal pairs [286]. For carbon- based (e.g., diamond, graphite/graphene, diamond-like coatings, nanotubes) and other covalent systems, a series of FFs has been developed, all based on the bond order concept originally formulated by Pauling [287]. Examples include the Finnis-Sinclair [288], Tersoff [289] and Brenner [290]

potentials, as well as more recent derivations such as the Adaptive Intermolecular Reactive Empirical Bond Order (AIREBO) [291] and ReaxFF [292] FFs. These all share the common assumption that it is possible to properly model the strength of a chemical bond on the basis of the bonding environment, thus considering the number of bonds and, if necessary, bond lengths and bending angles. Such kinds of potentials have been successfully used to investigate the tribological properties of different systems, including the interaction between diamond samples [293-295], the frictional behavior of corrugated nano-structured surfaces [296], the wear mechanisms of tungsten-carbon systems [297], friction and adhesion properties of carbon nanotubes and polymers [298,299], and tribochemical reactions on silicon/ silicon oxide interfaces [300,301].

Another class of potentials used in tribology are non-reactive FFs (see, e.g. [302-305]). This class of potentials is often employed to model intramolecular interactions in organic molecules and contains several two-, three- and four-body terms (usually including LJ, electrostatics, bond stretching, angle bending and torsional parts). As already mentioned, despite the simplicity and relatively low computational cost of such non-reactive FFs, a fixed topology has to be provided as an input for an MD simulation, thus preventing the possibility of investigating tribochemical reactions or events that require the breaking/formation of chemical bonds in general. Instead, when modeling tribochemistry, MD techniques [305-307] or quantum calculations (using Density Functional Theory, DFT) [308] are used to study atom motion during friction or chemical reactivity, respectively. To combine both types of information, reactive force-field MD [309], ab initio MD techniques [272] or tight-binding coupled with MD [310] techniques have also been used to extract in situ information of interfacial material behavior. A deeper insight of the local electronic and geometric characteristics is required to capture subtleties that a molecular mechanical description cannot represent. Indeed, quantum mechanical approaches have been used toward this aim, e.g., [311], focusing on the theoretical modeling of a specific stoichiometry and chemical composition. Tribochemistry is discussed in more detail in §3.9.2.

Classical MD –especially when calculating and tracking the kinematics of all atoms (all-atom MD) as opposed to aggregates of these (united-atom or coarse-grained MD)– require significant computational resources, meaning that the method is usually reserved for systems of relatively small sizes (less than a cubic micrometer) studied for a short time (less than a microsecond), even with today’s increased capabilities. In what is essentially a boundary element method, Green’s Function MD (GFMD) [312]

integrates out “all internal (harmonic) modes of an elastic body, […] leading to effective interactions of those atoms whose degrees of freedom couple to an external force.” In this manner, “the full elastic response of semi-infinite solids is incorporated so that only the surface atoms have to be considered in molecular dynamics simulations” [313]. GFMD is being used extensively in the study of tribological systems, including in the recent contact-mechanics challenge summarized in §3.5.

**2.6. Multiscale modeling: concurrent and hierarchical schemes **

By multiscale modeling, one refers to a technique in which two (or more) different models related to different scales (or different matter descriptions) interact, i.e. exchange data, in a way that enhances the information that can be obtained about the modelled phenomenon. Contact between rough surfaces with geometrical features present on multiple scales, starting from the shape of contacting solids down to the atomic fluctuating nature of the “surface” at the nanoscale, is an example of a spatially

15

multiscale problem. Earthquakes, on the other hand, constitute the most characteristic example of a temporally multiscale problem, in which the stresses building up in the earth’s crust for many years are released within seconds inside the fault zone, giving rise to seismic waves. In general, spatially multiscale problems are much more complicated to model than temporally multiscale ones, as time is only a one-dimensional quantity. Consider, for example, a multiscale contact problem between rough surfaces: this can be solved using either a classical model (FEM, BEM and so on, as discussed in

§2.2), e.g., as in [119], or a multiscale model, e.g., as in [314]. In such a multiscale model of rough contact, the upper scale model (e.g., treated with the FEM) determines the state (for example, the contact pressure) for the microscale (e.g., treated with the BEM), whereas the microscale provides the upper state with some properties of the contact interface such as, for example, the contact stiffness, contact area, friction, etc.

Having been generalized by many authors, the problem of multiscale rough contact inspired numerous theoretical and computational studies aimed at understanding the role of roughness at different scales of observation; see, e.g., [112,314-317] among many others. Recently, the topic has gained renewed interest with the increased potential of MD in studying nanoscale contact problems [263,276,318,319]

that unveil interesting mechanisms of contact interactions occurring at the nanoscale. While the advent of MD opened new challenges due to the still limited time and size scales of the simulations that can be performed with the aid of supercomputers, it has also revealed new opportunities for the use of various multiscale approaches.

An important question in multiscale modeling is the following: how to identify which spatial and temporal scales and mechanisms are relevant for understanding the phenomena to be modelled? A simple recipe would be to start with a simpler model, based on a single scale and uncoupled physical processes, and then adaptively introduce additional scales to permit coupled multiscale-multiphysics considerations, whenever and wherever these are needed, until the simplest possible model is obtained.

Scale, in this context, does not only refer to the spatial and temporal dimensions, but also to the different computational models relevant to different scales. Inevitably, some multiscale coupling also implies multiphysical coupling as, for example, in the case of coupling mechanical FEM with classical MD in which thermal oscillations are inherent to the model [320]. However, this simple recipe can be often ineffective as it depends on the ability of the “user” to add the right details at the right scale and may lead to the neglect of important information flow across the scales.

In tribological models, key processes are usually localized in a thin interface layer, but have important implications or can even fully control the macroscopic behavior of the system. In this light, the interfacial laws of friction, wear, heat and electrical transfer, as well as other relevant phenomena can be obtained with microscale models for use in macroscale ones. In terms of accuracy, one can determine two levels in this hierarchical approach: 1) the microscale model is assumed to not affect the macroscale state, in which case the microscale data can be obtained by simply post-processing the macroscale results; 2) the microscale model affects the macroscale state and, thus, the constitutive interface model has to be directly included in the latter scale. For most applications in which scale separation between the micro- and the macroscales exists, a hierarchical multiscale model is acceptable and the relevant question would be: when would a finer and truly multiscale model –i.e., one which requires stronger scale coupling– be needed? Normally, a finer model is required when no scale separation exists, as is normally the case for surface roughness. Such models, dealing with concurrent multiscale coupling are in general much more complex and can hardly be used to obtain statistically meaningful results; see, e.g., [204,320-322]. At the same time, finer models can be used for rare-event simulations and are of high importance in understanding the physics of certain phenomena happening in contact interfaces such as dislocation interaction with free surface in contact

16

interfaces [323,324], ballistic heat diffusion through small contact spots [320,325], partial slip conditions in lubrication at the molecular level [326], and so on. Most such phenomena can be studied at a single relevant scale and integrated at a bigger scale in a hierarchical manner.

In the case of plastic deformations occurring, for instance, during sliding motion between two metallic surfaces, many dislocations are nucleated at the surfaces and under maintained load may travel long distances. In an MD simulation, the small size of the domain will artificially trap them and create artificial hardening, which should occur in very thin coatings. In order to address this issue, advanced concurrent coupling strategies are being developed where dislocations can be passed to a continuum representation [327,328]. In three dimensions, dislocations are line networks, so that a dislocation may cross the coupling interface. Such hybrid dislocations should behave as single dislocation structure, which requires the use of reciprocal boundary conditions and may significantly increase the complexity of coupling strategies.

Another important aspect to consider is the possibility to perform concurrent coupled simulations where atomistic and molecular details need to be captured near the wall in lubricated contacts when the fluid film is larger than the Root Mean Square (RMS) composite surface roughness; this is particularly useful, for example, when slip at the wall or atomistic details of the surface topography must be explicitly modelled. In this case, MD-continuum coupling strategies involve the transfer of information between MD and CFD, and particular care must be taken when the two descriptions merge [329,330]; a number of schemes exist to achieve this [331-333].

Finally, comparison with experimental data is of crucial importance for all types of models, and multiscale ones are not an exception. Difficulties here arise from the fact that it is not always possible to reproduce the relevant scales for the application/model in the lab. For example, the friction of rocks (as well as their fracture) is a very scale-dependent phenomenon [334] that is intimately linked to the probability of presence of critical defects in a given volume. The related key question in this example would be: what are the features of real earthquakes, which can be reproduced in the lab? Also, can multiscale models tuned at the lab scale, e.g. [335], be used at earthquake scales? Further research on scale separation in contact interactions is required to guide the choice of the most appropriate computational method preserving the accuracy of the description of a given physical problem while considering the effect of inherent uncertainties.

**3. Research themes in tribology **

The problem of normal contact between rough surfaces has been studied extensively –for example, the reader is referred to a recent paper on a contact-mechanics challenge whose results are summarized in

§3.5– and can be considered to be well understood, but almost all other issues in tribology remain open for future research. While different theories, techniques and models used to investigate these issues were reviewed in §2, this section introduces active topics for modeling research in tribology. As a foreword, let us emphasize that, since the global forces acting on an interface are integral quantities along the interface (for example, the friction force is the integral of the shear stress over the contact area), various models can predict rather similar forces using different assumptions. Comparisons of models to experiments are therefore necessary, not only in terms of global forces but also in terms of local measurements, for instance, of temperature, strains or the real area of contact. Multiple successful examples of such comparisons can be found in the literature [336-346]. Local measurements become increasingly accessible due to the miniaturization of local probes and the development of full-field evaluation techniques like Digital Image Correlation (DIC) [347] or infrared imaging [348]. Imaging techniques are especially interesting for performing local measurements at a